Download presentation

Presentation is loading. Please wait.

Published byHaley McFarland Modified over 4 years ago

1
Max-Planck-Institut für Plasmaphysik EURATOM Assoziation Interaction of nitrogen plasmas with tungsten Klaus Schmid, A. Manhard, Ch. Linsmeier, A. Wiltner, T. Schwarz-Selinger, W. Jacob, Stephan Mändl

2
K. Schmid 2009 Introduction Summary Outline Experiment & Results N accumulation & sputtering of W Nitride phase formation

3
K. Schmid 2009 Introduction ASDEX Upgrade (now full W) experiments show performance increase for N 2 seeding in the divertor compared to Ne or Ar [1]: Why N and W ? [1] A. Kallenbach, et. Al. Nuclear Fusion 49 (2009) 045007 Question: Influence of nitrogen ions on tungsten PFCs ? Sputtering of tungsten by nitrogen Nitrogen accumulation in tungsten Thermodynamics and thermal stability of the tungsten-nitrogen system Perform experiments on: + Improved energy confinement + Smaller ELMs N 2 gas puffing is used for edge plasma cooling in high-Z PFC fusion experiments

4
K. Schmid 2009 Experiment & Results N-accumulation and Sputtering of W by N grid Sample holder U DC, bias ECR plasma ion source with freely expanding plasma beam Homogenous irradiation of samples Ion energy by DC biasing up to 500V Water cooled sample holder Ion flux & energy distribution measured by retarding field analyzer: 3 to 4x10 18 N y + (m -2 s) Molecular ion distribution measured by plasma monitor Dominantly N 2 + ions PLAQ Samples W Cu Si PVD tungsten layer ~ 500 nm PVD copper interlayer ~100 nm stress relief Silicon substrate well-defined surface for RBS analysis Implantation setup

5
K. Schmid 2009 Experiment & Results N-accumulation and Sputtering of W by N N 2 plasma flux and composition Retarding field analyzer measurements Flux :3 - 4 x 10 14 N 2 + / cm 2 s in main peak Most ions have energy corresponding to bias Plasma monitor measurements Plasma dominated by N 2 + ions N 3 + ions occur at highest pressures ~1Pa N + ions maintain constant level with pressure Implantations were performed at 0.25 Pa 90% N 2 +

6
K. Schmid 2009 Experiment & Results N-accumulation and Sputtering of W by N Measuring N accumulation in W by nuclear reaction NRA with 3.8 MeV 3He Reaction used: 14N ( 3He, p ) 16O Sensitivity: 10 15 N/cm 2 0.13 cts/ C Peak integral of p1 + p2 protons is evaluated to obtain the N areal density Measuring W sputtering via thickness change of W layer Rutherford backscattering (2.3 MeV 4He) Yields tungsten layer thickness Sensitivity: 10 12 W atoms / cm 2

7
K. Schmid 2009 Experiment & Results N-accumulation and Sputtering of W by N Implantation in plasma ion source PlaQ Low energy ions Sample temperature room temperature Quick saturation of retained N amount TRIDYN calculations predict similar levels Diffusion of N in W low (similar to C in W) N accumulation controlled by the implantation range For our low implantation energies one expects accumulation in the range of:

8
K. Schmid 2009 Experiment & Results N-accumulation and Sputtering of W by N Sputter yield of W by N from an N 2 plasma Sputter yield is much lower that expected from static TRIM Accumulation of N in W surface reduces partial sputter yield Good agreement between dynamic TRIM and experiment (dyn. Surface evolution) For Ne no accumulation in W surface Ne Sputter yield matches static TRIM N accumulation in W surface shields W from erosion by N Could partly be the reason for the good AUG performance with N-puffing

9
K. Schmid 2009 Experiment & Results Nitride phase formation Bombardment of W by 3keV N ion beam XPS analysis to identify nitride formation Literature data on W4f shift due to nitride formation varies strongly We find a shift of 0.45eV for nitride peaks. (lies within the literature data range) The intensity of nitride phase decreases with temperature

10
K. Schmid 2009 Experiment & Results Nitride phase formation W-N Phase diagram calculated by ThermoCalc TM Based on very little available data N 2 gas phase suppressed At ambient pressures WN instable above ~600K XPS measurements confirm thermodynamic modeling WN decomposes at high temperatures and N is lost as degassing N 2.

11
K. Schmid 2009 Plasma immersion ion implantation at IOM Leipzig 10 kV pulses Sample heated by pulses Implantation fluence comparable to plasma implantation Retained amount of N decreases with temperature above 650K Experiment & Results Nitride phase formation Decay above ~650K Nicely fits predictions by thermodynamic modeling As expected: Total accumulated amount higher than in our plasma implantation due to higher energies

12
K. Schmid 2009 Summary N accumulation quickly saturates once implantation range is filled with nitride phase Total amount of N is determined by N energy via the implantation range N accumulation in the surface leads to a reduction in the partial W sputter yield Advantage over noble gas seeding species XPS measurements of nitride fraction & measurements of total N amount indicate that the nitride decomposes at elevated temperatures This is line with thermodynamic calculations by ThermoCalc TM

Similar presentations

Presentation is loading. Please wait....

OK

Karolina Danuta Pągowska

Karolina Danuta Pągowska

© 2018 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google